Page:EB1911 - Volume 16.djvu/360

Rh conveniently used in the same manner as the three-pit system of liming, each wheel having three packs of skins through it before being thrown away. This paddling tends to make a bolder grain, as the skins are kept in continual motion, and work over one another. Some manufacturers finish the tannage with a mixture of sumach and oak bark; this treatment yields a less porous product. Others, when the skins are strained and in a semi-dry condition, apply neatsfoot or other oil, or a mixture of glycerine and oil, to the grain to lubricate it and make it more supple; the glycerine mixture is generally used for “chrome” leather, and will be discussed later under that head.

The skins tanned as above are largely dressed as morocco. Originally “morocco” was produced by the Moors in southern Spain and Morocco, whence the industry spread to the Levant, Turkey and the Mediterranean coast of Africa generally, where the leather was made from a species of sumach. Peculiarly enough, the dyeing was carried out before the tanning, with Roman alum as “mordant” and kermes, which with the alum produced a fine red colour. Such leather was peculiarly clear in colour, elastic and soft, yet firm and fine in grain and texture, and has long been much prized for bindings, being the material in which most of the artistic work of the 16th-century binders was executed. Now, in addition to the genuine morocco made from goat skins, we have imitation or French moroccos, for which split calf and especially sheep skins are employed, and as the appearance of morocco is the result of the style of graining and finish, which can now be imitated by printing or embossing machines, morocco can be made from all varieties of thin leather.

Great quantities of “Persian” (East India tanned) sheep and goat are now dressed as moroccos and for innumerable other purposes, the method being as follows: The goods are tanned with turwar bark and cassia bark, besides being impregnated with sesame oil, even to the extent of 30%. The first operation is to “strip” them of the oil and original tannage as far as possible, by drumming in a solution of soda; the soap thus formed is got rid of by thoroughly washing the goods, when they are “soured” in a weak bath of sulphuric acid to brighten the colour and remove iron stains, after which they are washed up and re-tanned by drumming in warm sumach, allowing about 4 oz. per skin. They are then slicked out, dried and are ready for dyeing.

The tanning of sheep and lamb skins differs very essentially from the tanning of goat and other leathers, mainly in the preparatory processes. As the wool is completely destroyed by lime, other methods have to be resorted to. The process usually practised is known as “sweating”; this consists of hanging the moist skins up in a warm, badly-ventilated chamber and allowing incipient putrefaction to set in. The chamber is always kept warm and saturated with moisture, either by means of a steam jet or water sprinklers. During the process large quantities of ammoniacal vapours are given off, and after two or three days the skins become slimy to the touch, and the wool slips easily; at this stage the goods are removed, for if the putrefaction goes too far the grain of the skin is irretrievably ruined. The wool is now “pulled” by pullers, who throw it into bins arranged to receive the different qualities; for one pelt may have three different grades of wool on it.

Other methods of dewooling are to paint the flesh with a solution of sodium sulphide, or cream of lime made with a solution of sodium sulphide; in either case the goods are piled flesh to flesh for an hour or so, and care is taken that the dewooling agent does not touch the wool. The pelt is then pulled and rapidly swilled in a stream of running water. The goods are now, in some yards, lightly limed to plump them superficially, by paddling in a milk of lime, and at this stage, or when the goods have been “struck through” with tan liquor, they are “degreased” either by hydraulic pressure or by benzene degreasing. This is to expel the oleaginous or fatty matter with which sheep skins are richly impregnated; the average yield is about 4 oz. per skin. The tannage is carried out in much the same way as for goat skins, the goods being started in old acid bark liquors; the general tannage consists of sumach and bark.

Basils are sheep skins tanned in various ways. English basils are tanned with oak bark, although, as in all other leathers, inferior tannages are now common; Scotch basils are tanned with larch bark, Australian and New Zealand basils with mimosa bark and Turkish basils with galls. The last are the commonest kind of skins imported into Great Britain, and are usually only semi-tanned. Roans are sumach-tanned sheep skins.

Skivers are the grain splits of sheep skins, the fleshes of which are finished for chamois leather. The goods are split in the limed state, just as the grains are ready for tanning, and are subsequently treated much as sumach-tanned goat skins, or in any other convenient way; the fleshes, on the other hand, go back into the limes, as it is necessary to get a large quantity of lime into leather which is to be finished as chamois.

Russia Leather was originally a speciality of Russia, where it was made from the hides of young cattle, and dressed either a brownish red or black colour for upper leather, bookbinding, dressing-cases, purses, &c. It is now made throughout Europe and America, the best qualities being obtained from Austria. The empyreumatic odour of the old genuine “Russia” leather was derived from a long-continued contact with willow and the bark of the white birch, which contains the odorous betulin oil. Horse hides, calf, goat, sheep skins and even splits are now dressed as “Russia leather,” but most of these are of a decidedly inferior quality, and as they are merely treated with birch bark oil to give them something of the odour by which Russia leather is ordinarily recognized, they scarcely deserve the name under which they pass. The present-day genuine Russia leather is tanned like other light leathers, but properly in willow bark, although poplar and spruce fir barks are used. After tanning and setting out the goods are treated with the empyreumatic oil obtained by the dry distillation of birch bark. The red colour commonly seen in Russia leather is now produced by aniline colours, but was originally gained by the application of an infusion of Brazil wood, which was rubbed over the grain with a brush or sponge. Some time ago Russia leather got into disrepute because of its rapid decay; this was owing to its being dyed with a very acid solution of tin salts and cochineal, the acid completely destroying the leather in a year or two. The black leather is obtained by staining with logwood infusion and iron acetate. The leather, if genuine quality, is very watertight and strong, and owing to its impregnation with the empyreumatic oil, it wards off the attacks of insects.

Seal Leathers, &c.—The tannage of seal skins is now an important department of the leather industry of the United Kingdom. The skins form one of the items of the whaling industry which principally centres in Dundee, and at that port, as well as at Hull and Peterhead, they are received in large quantities from the Arctic regions. This skin is that of the white hair seal, and must not be confused with the expensive seal fur obtained from Russian and Japanese waters. These white hair seal skins are light but exceedingly close in texture, yielding a very strong tough leather of large area and fine bold grain, known as Levant morocco. The area of the skins renders them suitable for upholstery work, and the flesh splits are dressed in considerable quantity for “japanned” (“patent”) leather and “bolsters,” which are used to grain other skins on, the raised buff affording a grip on the skin being grained and thus preventing slipping. When the skins arrive in the tanyard (generally lightly salted) they are drummed in old drench liquors until soft, dipped into warm water and “blubbered” with a sharp knife; they are then alternately dipped in warm water and drummed several times to remove fat, after which they are heavily limed, as they are still very greasy, and after unhairing and fleshing they are heavily puered for the same reason. The tannage takes about a month, and is much the same as for other leathers, the skins being split when “struck through.”

Alligator leather is now produced to some extent both in the United States and India. The belly and flanks alone are useful. There are no special tanneries or processes for dressing the skins. Layers are not given. The leather is used mostly for small fancy goods, and is much imitated on sheepskin by embossing.

Snake and frog skins are also dressed to some extent, the latter having formed a considerable item in the exports of Japan; they are dressed mostly for cigar cases and pocket books. The general procedure is first to lime the goods and then to remove any scales (in the case of snake skins) by scraping with an unhairing knife on a small beam, after which the skins are bated and tanned in sumach by paddling.

A considerable amount of leather is now produced in Australia from the skins of kangaroo, wallaby and other marsupials. These skins are both tanned and “tawed,” the principal tanning agents being mimosa bark, mallet bark and sugar bush, which abound in Australia. The leather produced is of excellent quality, strong and pliable, and rivals in texture and appearance the kid of Europe; but the circumstance that the animals exist only in the wild state renders them a limited and insecure source of leather.